An Investigation to Nonlinear Elastic Behavior of
Peri-cardium Using Uniaxial Tensile Test
M. Arman, K. Narooei∗
Department of Materials Science and Engineering, K. N. Toosi University of Technology, Tehran, Iran.
Received 2016.04.06 Received in revised form 2016.06.11
nonlinear elastic behavior strain energy function Green material Cauchy material
In this paper, the nonlinear elastic behavior of pericardium of human, canine, calf and ostrich was studied. For this purpose, the mechanical behavior was investigated from two viewpoints of the Cauchy and Green elastic materials. Firstly, the experimental data were fitted by Cauchy elastic stress equation. The results showed that the response of Cauchy elastic materials was not fitted with the experimental data appropriately. Secondly, the Green elastic materials were studied by assuming strain energy functions for the mechanical response of the samples. For this purpose, the exponential-exponential, power law-power law, and exponential-power law energy functions were investigated by mathematical programming. It was observed that all energy functions were fitted with the experimental data accurately, especially the power law-power law function. Finally, it was observed that the Green elastic materials theory was more appropriate for studying the mechanical behavior of pericardium by comparing the experimental and theoretical results.
Pericardium is a tough double layered membrane cov-ering the heart. It plays an important role in the nor-mal cardiac work. Its major functions include: main-tenance of adequate cardiac position, separation from the surrounding tissue of the mediastinum, protec-tion against ventricular dilataprotec-tion, maintenance of low transmural pressure, facilitation of ventricular interde-pendence and arterial filling. Given the position and role of pericardium, it is necessary to study the behav-ior of it in the face of environmental factors. Noort et al. introduced a new experimental technique to study the effects of glutaraldehyde and formaldehyde on the stress-strain response of bovine pericardium . Also, Chew et al. investigated canine pericardium behavior under biaxial loading conditions using a new quantita-tive method . Maestro et al. compared the mechan-ical and chemmechan-ical behavior of glutaraldehyde-preserved ostrich pericardium as a novel biomaterial with bovine pericardium, observing that the tensile strength of
os-trich pericardium was higher than bovine pericardium . Daar et al. investigated the effects of penetrating ionising photon radiation on the mechanical properties of pericardium in the uniaxial tensile test. In this re-search, it was concluded that UTS was reduced to the dose of 80 Gy . Paez et al. studied the mechanical behavior of calf, pig, and ostrich pericardium in unsu-tured and suunsu-tured states using a statistical method; it was concluded that ostrich pericardium had suitable mechanical resistance, relative to pig and calf peri-cardium, and it could be used as new biomaterials in the fabrication of bioprosthesis . Claramunt et al. studied the fatigue behavior of young ostrich peri-cardium and presented the relationship between the number of cycles until the failure of each sample and the maximum pressure by the least square method . Cohn et al. compared the mechanical behavior of ca-nine, human, and bovine isolated pericardium in tensile testing . Zioupos and Barbenel, on the other hand, proposed a constitutive law for the investigation of the mechanical behavior of native bovine pericardium in
∗Corresponding author: Keivan Narooei (Assistant Professor)
E-mail address: firstname.lastname@example.org
uniaxial and biaxial tensile tests . Lee and Bough-ner conducted uniaxial tensile tests on the human and canine pericardium tissue to compare the viscoelastic response, showing that the human pericardium, in con-trast to canine pericardium, indicated a greater viscous behavior . Gundiah et al. studied the strain energy functions (SFE) for arterial elastin and concluded that Mooney-Rivlin model did not cover the arterial elastin behavior. Thus, they proposed an orthotropic materi-als model . Zulliger et al. proposed a new SFE by expanding the model developed by Fung and Holzapfel model, characterizing the fraction of both elastin and collagen on rat carotids . Also, Zulliger and Ster-giopulos studied the main structural factors of the hu-man thoracic aorta using the strain energy function. In this research, it was shown that the changes in the mechanical behaviour of aorta could not be included in the elastic constants of elastin and collagen by in-creasing the age . Kulkarni et al. studied the bovine pericardium and porcine brain tissue using transversely hyperelastic materials including matrix and reinforced fibres, by considering the large deformation at high strain rates. The matrix part was simulated using the Neo-Hookean strain energy function and in the fibres part, the polyconvex polynomial model was used . Pavan et al. presented a constitutive model consid-ering the incompressibility, large strain and time de-pendency for pericardial tissue in human . Miller proposed a three-dimensional hyper-viscoelastic con-stitutive model for kidney and liver tissue on the basis of in vivo experiments . Gao et al. proposed two new exponential/logarithmic and Ogden based consti-tutive models for the FE analysis of porcine liver tissue. These models captured the simple tension, compression and pure shear experimental data . Veljkovic et al. investigated the mechanical behavior of porcine aorta under extension-inflation tests using different hyper-elastic models. They studied the Fung strain energy function in two dimensions and polyconvex model in three dimensions, concluding that the two-dimensional model had a good agreement with the experimental data, but three-dimensional model did not represent a proper mechanical response in the axial direction of artery . Ogden et al. investigated the mechanical behavior of rubber materials using isotropic stored en-ergy functions in the incompressible state, by the op-timization of material parameters with the nonlinear least square analysis . Darijani et al. proposed the novel strain energy functions based on Logarithmic, ex-ponential, power law and polynomial equations. It was shown that the proposed models demonstrated a good agreement with the experimental data .
In this research, the nonlinear elastic behavior (Green and Cauchy elastic materials model) of the pericardium of calf and ostrich was investigated. For this purpose, the Cauchy elastic materials were presented as materi-als with no zero energy in the closed deformation cycle
and the Green elastic materials were introduced with the specific strain energy functions. The coefficients of each constitutive equation were calculated for the best correlation with the experimental data.
2. Nonlinear Elastic Model
In most metals, the elastic part of stress-strain curve is linear, but the elastic behavior is usually nonlinear in polymers, elastomers, and soft tissue. Therefore, a suitable constitutive equation is required to model nonlinear behavior. These constitutive equations are classified into the following two categories: Cauchy and Green elastic materials. These two categories are de-scribed in the next sections.
2.1. Cauchy Elastic Materials
In the Cauchy elastic materials, stress does not depend on the history of deformation, but the work done by the stress depends on the deformation path. In these materials, the general form of constitutive equation can be written as :
σ=H(B) +ψ0I+ψ1B+ψ2B2 (1)
where αis refers to the scalar invariants and I is the second order identity tensor. By considering the left Cauchy-Green tensor (B=V2), Eq. (3) can be rewrit-ten as :
σ=H(B) =ψ0I+ψ1B+ψ2B2 (2)
where ψ0, ψ1 and ψ2 are the scalar invariants of B.
Since a tensor should satisfy the characteristic equa-tion, the Cauchy elastic material constitutive equation is written by considering the hydrostatic pressure as a constraint :
In simple tension, σ1 = σ ̸= 0 and σ2 = σ3 = 0.
If λ1, λ2, and λ3 represent the principal stretches for
incompressible materials in the uniaxial tension, the relation λ1 = λ and λ2 = λ1 = λ−0.5 can be
as-sumed. Therefore, by using Eq. (3) and condition σ2 = σ3 = 0, the hydrostatic pressure can be
calcu-lated asp= φ1
λ +φ2λ. Thus, Eq. (3) can be expressed
( 1 λ2
If a material obeys the Cauchy elastic response, the ex-perimental data should be fitted with the Eq. (4). In the next section, the Green elastic response of material will be discussed.
2.2. Green Elastic Materials
other words, in the Cauchy materials, only the stress is independent of loading path, but in the Green ma-terials, the work is also independent of load path in addition to the stress . These materials are char-acterized by a strain energy function with necessary conditions . So, according to the material symme-tries and strain energy functions conditions , it can be written [18,21]:
W(λ1, λ2, λ3) =W(λ1) +W(λ2) +W(λ3) (5)
As mentionedλ1=λand λ2 =λ3=λ−0.5 for
incom-pressible materials in the uniaxial tension, Eq. (5) can be expressed:
W(λ) =W(λ) +W(λ6−0.5) +W(λ−0.5) (6)
The principle Lagrangian stresses are obtained by the derivative of strain energy function with respect to stretches [22, 23, 28]:
Also, the principle Cauchy stresses can be obtained as [22,23,28]:
In Eq. (8), “i” is not a dummy index. Many strain energy functions such as Mooney-Rivlin, Ogden, and Neo-Hookean have been used in the recent investiga-tions, but in this study, the robust novel strain energy functions proposed by Darijani and Naghdabadi were used . The following functions, which include power law and exponential terms, satisfy the strain energy function conditions. By combining these functions, 16 strain energy functions can be derived. In this paper, only exponential (exp-exp), exponential-power law (exp-pow) and exponential-power law-exponential-power law (pow-pow) strain energy functions have been investigated . Generally, the strain energy function for multiax-ial loading can be stated as [22,23]:
1. The exponential-exponential function (exp-exp):
Bk[exp(nk(λ−i 1−1))−1] (9)
2. The exponential-power law function (exp-pow):
3. The power law-power law function (pow-pow):
Ak(λmi k−1) +
where Ak, Bk, mk and nk are constants obtained from fitting these equations to the experimental data. Also, λis refers to principal stretches in different di-rections. It should be noted that there are two sum-mations in the above equations. The first summation provides the positive infinity at the large deformation case and the second one causes the negative infinity at the singularity case.
In this paper, the sum of squared errors (SSE) was used for the description of the accuracy of the models. Actually, SSE represents the difference between the ex-perimental valuesxexpi and the modelled (theoretical) valuesxtheo
i . It was calculated as follows:
(xexpi xtheoi )2 (12)
3. Results and Discussion
The mechanical behavior of pig, calf, and ostrich peri-cardium in sutured and unsutured states, with Gore-Tex at 45◦ and 90◦, cut in the dimensions of 12×2 cm2 was compared with the uniaxial tensile test
re-sults obtained by Paez et al. . The stress-strain experimental data of the uniaxial tensile test for os-trich and calf pericardium were adopted from Paez et al. . The experimental stress-strain data of human and canine pericardium with the size 3×3 cm2in the uniaxial tensile were adopted from Lee and Boughner .
elastic material stress did not fit the uniaxial tensile test data for ostrich, canine and human and only calf pericardium data could be fitted precisely. It should be noted that the range of stress axes in Fig. 1 was not the same for the cases of calf and ostrich. Therefore, as it can be seen in Table 1, the SSE of fitting for the case of ostrich pericardium was higher than that of calf pericardium.
The energy of deformation can be calculated as :
W = ∫ λ
The results of the calculated energy of stress curves, as shown in Fig. 1, could be seen in Fig. 2. Since the coefficients of data fitting were calculated based on the stress-stretch/strain curves of the uniaxial tension tests, there was no guarantee that the energy func-tions could be fitted to the experimental energy data
with these coefficients. Also, there was no constraint for energy to be non-negative during the deformation. According to Figs. 2b and 2d, it could be seen that not only did the theoretical energy function not fit the experimental data, but also the negative energy was generated in the limiting range of stretches, which was not a physical result. Additionally, there was a poor correlation between the fitted energy curves and the experimental data for other cases.
Coefficients of the stress response in the Cauchy elastic materials (Eq. (4)).
Case φ1(MPa) φ(MPa) SSE
Calf 56.66 58.88 0.01097
Ostrich 539.4 608.4 235.3
Canine 22.65 22.78 45.44
Human 16.51 18.11 44.17
Fig. 2. Energy of Cauchy elastic response and the experimental data: (a) calf pericardium, (b) ostrich pericardium, (c) canine pericardium, and (d) human pericardium.
As the Cauchy elastic material does not ensure that the energy is zero in the close cycle of deformation [22,23], the Green elastic material was investigated here. From the viewpoint of Green elastic materi-als, the energy was calculated from the tensile stress-elongation curves as the surface under the curve of the experimental data. Then, the strain energy functions of exp-exp, pow-pow and exp-pow were fitted with the experimental data. The results of choosing two terms for each of the series in Eq. (9), (10), and (11) can be seen in Fig. 3. The best fitting coefficients and SSE for human, canine, calf and ostrich in the case of Green elasticity are demonstrated in Table 2. The stress-stretch plots have been presented in Fig. 4, using Eq. (8).
In surgical operations, the soft tissue could be sub-jected to various modes of loading such as pure shear, biaxial and tension; therefore, coefficients of data fit-ting according to simple tension should capture the pure shear and biaxial data [16, 22]. In this research, pure shear and biaxial data were not available, but
the-oretical biaxial and pure shear stresses were calculated. According to Fig. 3, it could be observed that all functions, such as exp-exp, exp-pow and pow-pow func-tions, covered the uniaxial tension data. Also, it could be deduced that pow-pow function had a minimum value of SSE, as can be seen from Table 2, and it was better than exp-exp and exp-pow functions.
Coefficients of the strain energy functions in the Green elastic materials.
Calf(exp-exp) Ostrich(exp-exp) Canine(exp-exp) Human(exp-exp)
A1(MPa) 0.02275 10.35 −2.015×10−3 −2.639×10−3
A2(MPa) 2.539 0.5509 2.004×10−3 1.166×10−3
B1(MPa) 0.2031 300.5 1.241×10−3 8.412×10−3
B2(MPa) −20.73 −7670 7.455×10−3 6.771×10−3
m1(MPa) 3.122 3.596 5.02×10−2 2.309×10−2
m2(MPa) 3.049 7.898 5.111×10−2 2.804×10−2
n1(MPa) 7.456 1.847 9.999×10−3 6.378×10−3
n2(MPa) 0.9943 0.1937 3.243×10−3 6.223×10−3
SSE 1.848×10−4 0.06649 3.355×10−5 10−5
Calf(exp-pow) Ostrich(exp-pow) Canine(exp-pow) Human(exp-pow)
A1(MPa) 60.77 8.696 3.594×10−2 −3.081×10−3
A2(MPa) 75.26 0.3304 1.222×10−5 1.634×10−3
B1(MPa) 2.056 49.11 4.446×10−3 1.177×10−2
B2(MPa) -9.154 -4692 −1.286×10−2 3.887×10−4
m1(MPa) 0.372 4.725 7.175×10−3 2.364×10−2
m2(MPa) 0.3679 0.002812 7.605×10−2 2.75×10−2
n1(MPa) 7.963 4.316 3.103×10−2 7.685×10−3
n2(MPa) 4.608 0.4916 2.197×10−2 4.236×10−4
SSE 6.413×10−5 0.05812 2.445×10−5 9.955×10−6
Calf(pow-pow) Ostrich(pow-pow) Canine(pow-pow) Human(pow-pow)
A1(MPa) 66.24 0.2284 −5.25×10−3 −1.185×10−3
A2(MPa) 46.94 10 1.742×10−3 4.062×10−4
B1(MPa) 3.435 1.622 4.61×10−3 1.126×10−2
B2(MPa) −13.54 −5815 6.528×10−2 4.677×10−4
m1(MPa) 0.9189 12.46 2.889×10−2 2.763×10−2
m2(MPa) 0.9168 2.167 4.113×10−2 3.493×10−2
n1(MPa) 7.335 11.98 9.087×10−3 7.166×10−3
n2(MPa) 4.511 0.2263 4.897×10−3 5.677×10−4
Fig. 4. Experimental data [5,9] and stress-stretch curves of: (a-c) exp-exp, exp-pow, and pow-pow stress response of calf pericardium, (d-f) exp-exp, exp-pow and pow-pow stress response of ostrich pericardium, (g-i) exp-exp, exp-pow and pow-pow stress response of canine pericardium, and (j-l) exp-exp, exp-pow and pow-pow stress response of human pericardium.
It should be noted that the stress response of a nonlinear hyperelastic strain energy is not well-known a priori. Regarding this, in a new hyperelastic strain energy, the stability, sensitivity and stress response in different loading paths and material constants should be investigated [18,26-28]. In this regard, as can be seen in Figs. 3 and 4, the biaxial stress state was dif-ferent for exp-exp and exp-pow hyperelastic strain en-ergy. Therefore, if there is a new hyperelastic strain energy that represents instability, asymptote or sensi-tivity with respect to small changes in material con-stants, the strain energy model should be neglected or modified . Since the modelling of the mechanical behavior of pericardium is important for the design and fabrication of valve leaflets bio-prosthesis, optimization of surgical instruments and development of computer-based simulators for training surgical students [5,24], in a future work, finite element analysis of pericardium
will be studied using a novel hyperelastic constitutive pow-pow equation with the minimum error.
pow-pow, and exp-pow equations were obtained in the uniaxial tensile test. It was shown that the calculated energy functions had good fitting with the experimen-tal data. Also, through these functions, the pow-pow energy function had less error than other functions. In general, it was obvious that the Cauchy elastic materi-als theory could not predict the nonlinear mechanical behavior of pericardium tissue reasonably, as compared to the results of Green elastic materials. Furthermore, since the energy is zero in the Green elastic materials response in a close deformation path, this theory could be utilized in finite element analysis and among the proposed models, the pow-pow model seems to have the minimum error.
The authors would like to thank K. N. Toosi University of Technology, Tehran, Iran, for providing the financial support and research facilities used in this work.
 R.V. Noort, S.P. Yates, T.R.P. Martin, A.T. Barker, M.M. Black, A study of the effects of glutaraldehyde and formaldehyde on the mechani-cal behaviour of bovine pericardium, Biomaterials. (1982) 21-26.
 P.H. Chew, F.S.P. Yin, S.L. Zeger, Biaxial Stress-strain Properties of Canine Pericardium, J. Mol. Cell. Cardiol. (1986) 567-578.
 M.M. Maestro, J.O.N. Turnay, P. Fernandez, D. Suarez, J.M.G. Paez, S. Urillo, M.A. Lizarbe, E. Jorge-Herrero, Biochemical and mechanical behav-ior of ostrich pericardium as a new biomaterial, Acta. Biomater. 2 (2006) 213-219.
 E. Daar, E. Woods, J.L. Keddie, A. Nisbet, D. A. Bradley, Effect of penetrating ionising radiation on the mechanical properties of pericardium, Nucl. In-strum. Methods. 619 (2010) 356-360.
 J. M.G. Paez, E.J. Herrero, A.C. Sanmartin, I. Mil-lan, A. Cordon, M.M. Maestro, A. Rocha, B. Are-naz, J.L. Castillo-Olivares, Comparison of the me-chanical behaviors of biological tissues subjected to uniaxial tensile testing: pig, calf and ostrich peri-cardium sutured with Gore-Tex, J. Biomaterials. 24 (2003) 1671-1679.
 R. Claramunt, J.M.G. Paez, L. Alvarez, A. Ros, M.C. Casado, Fatigue behaviour of young ostrich pericardium, Mater. Sci. Eng. (2012) 1415-1420.
 D. Cohn, H. Younes, E. Milgarter, G. Uretzky, Me-chanical behaviour of isolated pericardium: species,
isotropy, strain rate and collagenase effect on peri-cardium tissues, J. Clin. Mater. (1987) 115-124.
 P. Zioupos, J.C. Barbenel, Mechanics of native bovin pericardium, J. Biomaterials. (1994) 374-382.
 J.M. Lee, D.R. Boughner, Mechanical properties of human pericardium. Differences in viscoelastic re-sponse when compared with canine pericardium., Circ. Res. (1985) 475-481.
 N. Gundiah, M.B. Ratcliffe, L.A. Pruitt, Determi-nation of strain energy function for arterial elastin: Experiments using histology and mechanical tests, J. Biomech. (2007) 586-594.
 M.A. Zulliger, P. Fridez, K. Hayashi, N. Stergiop-ulos, A strain energy function for arteries account-ing for wall composition and structure, J. Biomech. (2004) 989-1000.
 M.A. Zulliger, N. Stergiopulos, Structural strain energy function applied to the ageing of the human aorta, J. Biomech. (2007) 3061-3069.
 S.G. Kulkarni, X.L. Gao, S.E. Horner, R.F. Mart-lock, J.Q. Zheng, A transversely isotropic visco-hyperelastic constitutive model for soft tissues, Math. Mech. Solids. (2014) 1-24.
 P.G. Pavan, P. Pachera, C. Tiengo, A. Natali, Biomechanical behavior of pericardial human tis-sue: a constitutive formulation, Inst. Mech. Eng. H J. Eng. Med. (2014) 926-934.
 K. Miller, Constitutive modelling of abdominal or-gans, J. Biomech. (2000) 367-373.
 Z. Gao, K. Lister, D.J. Desai, Constitutive Model-ing of Liver Tissue: Experiment and Theory, Ann. Biomed. Eng. (2010) 505-516.
 D.Z. Veljkovic, V.J. Rankovic, S.B. Pantovic, M.A. Rosic, M.R. Kojic, Hyperelastic behavior of porcine aorta segment under extension-inflation tests fitted with various phenomenological models, Acta. Bioeng. Biomech. (2014) 37-45.
 R.W. Ogden, G. Saccomandi, I. Sgura, Fitting hy-perelastic models to experimental data, Comput. mech. (2004) 484-502.
 H. Darijani, R. Naghdabadi, M.H. Kargarnovin, Hyperelastic materials modelling using a strain measure consistent with the strain energy postu-lates, J. Mech. Eng. Sci. (2010) 591-602.
 R.W. Ogden, Nonlinear elastic deformation, Dover Publication, 1997.
 H. Darijani, R. Naghdabadi, Hyperelastic mate-rials behavior modeling using consistent strain en-ergy density functions, Acta. Mech. (2010) 235-254.
 M. Mansouri, H. Darijani, Constitutive modeling of isotropic hyperelastic material in an exponential framework using a self-contained approach, Int. J. Solids. Struct. (2014) 4316-4326.
 F.J. Carter, T.G. Frank, P.J. Davies, D. Mc Lean, A. Cuschieri, Measurements and modelling of the compliance of human and porcine, Med. Image. Ana. (2001) 231-236.
 M.W. Lai, E. Krempl, D. Ruben, Introduction to continuum mechanics, Elsevier. (2010).
 T. Beda, An approach for hyperelastic model-building and parameters estimation a review of con-stitutive models, Eur. Polym. J. (2004) 97-108.
 A.S. Gendy, A.F. Saleeb, Nonlinear material pa-rameter estimation for charcterizing hyperelastic large strain models, Comput. Mech. 25 (2000) 66-77.